Standard Recommended Practice for
Selection and Use of Emulsified Asphalts
AASHTO Designation: R 5-03 ASTM Designation: D 3628-01
AASHTO R 5-03 is identical to ASTM D 3628-01 except that all references to the ASTM standards contained in ASTM D 3628-01, listed in the following table, shall be replaced with the corresponding AASHTO standard.
Referenced Standards ASTM AASHTO D 977 M 140
TS-2a R 5-1 AASHTO
Designation: D 3628 - 01
Standard Practice for Selection and Use of Emulsified ~sphalts' This standard is issued under the fixed designation D 3628; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript epsilon (E) indicates an editorial change since the last revision or reapproval.
1. Scope 1.1 This practice covers the selection of emulsified asphalts
for various paving and allied uses. 1.2 This standard does not purport to address all of the
safety concerns, if any, associated with its use. I t is the responsibility of the user of this standard to establish appro- priate safety and health practices and determine the applica- bility of regulatory limitations prior to use.
2. Referenced Documents 2.1 ASTM Standards: D 8 Terminology Relating to Materials for Roads and Pave-
ments2 D 977 Specification for Emulsified Asphalt2 D 2397 Specification for Cationic Emulsified Asphalt2 D 35 15 Specification for Hot-Mixed, Hot-Laid Bituminous
3. Terminology 3.1 Dejinitions: 3.1.1 bituminous-aggregate applications-applications of
bituminous material to a prepared aggregate base or pavement surface followed by the application of aggregate.
3.1.2 bituminous-aggregate mixtures-a combination of bi- tuminous material and aggregate that is physically mixed by mechanical means, spread on the job site, and compacted.
3.1.3 bituminous applications-the application of sprayed bituminous coatings not involving the use of aggregates.
3.1.4 crack jiller-the bituminous material used to fill and seal cracks in existing pavements.
3.1.5 dense-graded aggregate-aggregate that is graded from the maximum size, down to and including filler, with the object of obtaining a bituminous mix with a controlled void content and high stability.
3.1.6 dust binder-a light application of bituminous mate- rial for the express purpose of laying and bonding loose dust.
3.1.7 fog seal-a light spray application of asphalt to an
' This practice is under the jurisdiction of ASTM Committee D04 on Road and Paving Materials and is the direct responsibility of Subcommitee D04.41 on Emulsified Asphalt Specifications.
Current edition approved Dec. 10. 2001. Published January 2002. Originally published as D 3628 - 78. Last previous edition D 3628 - 97.
'Annual Book of ASTM Standards, Vol04.03.
existing pavement as a seal to inhibit raveling, or seal the surface, or both.
3.1.8 graded aggregate seal, n-a single surface treatment in which the aggregate is graded with little or no mineral filler, typically with a nominal maximum size of about 19 mm, and containing sufficient sand that the bituminous material will be required to penetrate upward into the aggregate cover; the nominal maximum aggregate size may vary depending on the course thickness desired and aggregate availability. It is an application method used in lieu of a chip seal to provide a lower cost road.
126.96.36.199 Discussion-In this case, nominal maximum size refers to the definition in Terminology D 8.
3.1.9 maintenance mix-a mixture of bituminous material and mineral aggregate applied at ambient temperature for use in patching holes, depressions, and distress areas in existing pavements, using appropriate hand or mechanical methods in placing and compacting the mix. These mixes may be designed for immediate use or for use out of a stockpile at a later date without further processing.
3.1.10 mixed-in-place-the procedures by which the bitu- minous material and mineral aggregrate are mixed on the job site by means of travel plants, blade mixing, or other special road-mixing equipment.
3.1.1 1 mulch treatment-a spray application of bituminous material used to temporarily stabilize a recently seeded area. The bituminous material can be applied to the soil or to a straw or hay mulch as a tie-down.
3.1.12 multiple surface treatment-two or more single sur- face treatments placed one on the other. The maximum aggregate size of each successive treatment is usually one half that of the previous one, and the total thickness is about the same as the nominal maximum size aggregate particles of the first course.
3.1.13 open-graded aggregate-aggregate containing little or no mineral filler and in which the void spaces in the compacted aggregate are relatively large.
3.1.14 pavement bases and surfaces-the lower or underly- ing pavement course atop the subbase or subgrade and the top or wearing course. Cold-laid mixtures that are bound together with liquid bitumens use either open or dense aggregate gradations.
3.1.15 penetration macadam-pavement construction using
Copyright 0 ASTM International, 100 Barr Harbor Drive. PO Box C700, West Conshohocken. PA 19428-2959. Unlled States
TS-2a R 5-2 AASHTO
esscntially one-size coarse aggregate which is penetrated in place by an application of high viscosity bituminous material followed by an application of smaller one-size coarse aggre- gate and thoroughly rolled. Procedure may be progressively repeated to reduce surl'ace voids as desired.
3.1.16 plant mix (cnlt1)-a mixture of bitunlinous material and mineral aggregate prepared in a central mixing plant and spread and corr~pacted at the job site when the mixture is at or ncar ambient temperature.
3.1.17 plnrrr mix (hot)-a mixture of bituminous material and mineral aggregate usually prepared in a conventional hot-mix plant or drum mixer at a temperature of not more than 127C and spread and compacted at the job site at a ternpera- ture above 93C.
3.1.18 prime coat-an application of low-viscosity bitumi- rlous material to an absorptive surface designed ro penetrate, bond, and stabilize this existing surface and to prornotc adhesion between it and the new super-imposed construction.
3.1.19 .sarid--a mineral aggregate material consisting of particles of rock passing a 4.75-mm sieve and only about 5 5% passing the 75-p.m sieve.
3.1.20 suntl seal-a bituminous-sand application to an ex- isting pavement surface to seal the surface and to function as a light-wearing course.
3.1.21 sur~dy soil-a n~atcrial consisting essentially of fine aggregate particles smaller than 2.00-mm sieve and usually containing ~naterial passing a 75-p.nl sieve. This material usually exhibits plasticity characteristics.
3.1.22 single-surface treutment (chip seu1)-Y wearing sur- face of bitunlinous matcrial and aggregate in which the aggregate is placed uniformly over the applied bituminous material in a single layer, the thickness of which approximates the nominal maximum size of the aggregate used.
3.1.23 slurry seal-a uniform application of a mixture of emulsified asphalt, fine aggregate, mineral filler, and water to an cxisting pavemcnt. Single or multiple applications may be used.
3.1.24 tack coat-an application of bitu~ni~lous matcr~al applied to an exlstlng, relatively nonabsorbent surface to provide a thorough hond between old and new surfacing.
3.1.25 treattiletlts and sealr-a bituminous aggregate appli- cation to any type of road or pavemcnt surface for the purpose of providing a wcarlng course. or a surfacc scal. or both.
4. Significance and Use 4.1 As indicated hy Specifications D 977 and D 2397,
ern~~lsifieil asphalts are classified by type (rapid mediurn or slow setting) and by grade within type (viscosity in the case of the rapid-setting type or characteristic of the residual asphalt in the case of the medium and slow-setting types). Selection for use of a particular type and grade is controlled by type of construction (whether an application or a mix type), properties of the mineral aggregate (both grading and mineral composi- tion), and environmental conditions during construction. For surface treatments and seals, emulsions are formulated to sel rapidly upon contact with the mineral aggregate or pavement surface. When used in mix types, slower breaking is required to allow time for mixing and laydown. If the mix aggregate is open graded without appreciable fines. a medium-setting emul- sion may be used that deposits a relatively hard asphalt. If the aggregate is dense-graded bur does not contain a large amount of very fine material (dust), a medium-setting emulsion with a soft residue may be a good choice. However, if the dense- graded aggregate contains a large amount of very fine mineral matter, a slow-setting emulsion may be required.
4.2 The recommendations in Table 1 should be considered only as a general guide for the selection of an e~nulsion for use. If the user is uncertain as to which to select for an intended use. the emulsion supplier should be contacted.
5. Keywords 5.1 emulsified asphalt; emulsion
TS-2a R 5-3 AASHTO
TABLE 1 General Uses of Emulsified Asphalt
N o m I-Only those gradzs o f emulsified asphalt in general use have been indicated herein. I t is possible that under certain variations of aggregates. or climatic conditions, or both, additional selections might be appropriate. Where the use o f emulsified asphalt for applications other than those listed i n the table are contemplated, the emulsion supplier should be consulted.